Applied Energy 99 (2012) 272–279
Contents lists available at SciVerse ScienceDirect
Applied Energy journal homepage: www.elsevier.com/locate/apenergy
Valorisation of spent coffee grounds as CO2 adsorbents for postcombustion capture applications M.G. Plaza, A.S. González, C. Pevida, J.J. Pis, F. Rubiera ⇑ Instituto Nacional del Carbón, INCAR-CSIC, Apartado 73, 33080 Oviedo, Spain
h i g h l i g h t s " Low-cost carbons with high CO2 uptake and selectivity are produced from coffee grounds. " Chemical activation is compared to physical activation. " KOH activation leads to carbons with higher CO2 uptake. " Coffee grounds activated with CO2 present higher CO2/N2 selectivity.
a r t i c l e
i n f o
Article history: Received 21 November 2011 Received in revised form 5 March 2012 Accepted 18 May 2012 Available online 22 June 2012 Keywords: CO2 capture Activated carbon Coffee residues
a b s t r a c t In this work spent coffee grounds from single-use capsules were used as the starting material for producing low-cost activated carbons. The activation conditions were selected and optimised to produce microporous carbons with high CO2 adsorption capacity and selectivity, thus with potential to be used as adsorbents in postcombustion CO2 capture applications. Two activation methods are compared: physical activation with CO2 and chemical activation with KOH. The ﬁrst method is considered less contaminant; however, leads to carbons with lower textural development and thus lower CO2 adsorption capacity than those obtained by activation with KOH. On the other hand, multicomponent adsorption cyclic experiments pointed out that the CO2/N2 selectivity of physically activated carbons is higher than that of chemically activated carbons. Ó 2012 Elsevier Ltd. All rights reserved.
1. Introduction Global emissions of carbon dioxide, considered to be the main contributor of global warming, increased by 45% between 1990 and 2010. Consumption of coal and natural gas (responsible for about 40% and 20% of total CO2 emissions, respectively) both grew in 2010 by 7% and cement production emissions (contributing 4% to the total) by 11%. Increased energy efﬁciency, nuclear energy and the growing contribution of renewable energy are not compensating for the globally increasing demand for power and transport. This illustrates the large and joint effort still required for mitigating climate change . IEA analysis suggests that Carbon Capture and Storage (CCS) will play a vital role in worldwide, least-cost efforts to limit global warming, contributing around one-ﬁfth of required emissions reductions in 2050 . Although lower energy penalties can be expected from applying carbon capture (CC) to an integrated gasiﬁcation combined cycle , this technology still seems a risky option to mitigate CO2 emissions of coal ﬁred power plants due to the cost associated to the ⇑ Corresponding author. Tel.: +34 985 11 90 90; fax: +34 985 29 76 62. E-mail address: [email protected]
(F. Rubiera). 0306-2619/$ - see front matter Ó 2012 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.apenergy.2012.05.028
integrated gasiﬁcation combined cycle (IGCC) technology . The main attractive of postcombustion CO2 capture is that it can be used for retroﬁtting existing facilities [5–7]. The CO2 present in the ﬂue gas produced at these sources can be separated for ulterior transport and storage by a number of techniques: absorption, adsorption, separation with membranes, cryogenic distillation, etc. [5,8,9]. Absorption with aqueous solutions of alkanolamines is a mature technology that has been extensively used in the sweetening of natural gas, and therefore is the natural extension for postcombustion applications, where CO2 is present at low partial pressures. However, the high energy penalty associated to the regeneration of the solvent (steam consumption accounts for over 50% of the overall operating costs ) has driven much research effort in the search of less energy-intensive alternatives. Adsorption, also a mature technology used industrially for the separation of air and the puriﬁcation of H2 among other applications [11,12], has been proposed as a candidate to reduce the cost associated to postcombustion CO2 capture [13–16]. Many adsorbents have been studied for CCS applications: zeolites, activated carbons, calcium oxides, hydrotalcites, MOFs, etc. [14,17–22]. The high pore volume and tailoring properties make MOF promising adsorbents for gas separation applications yet they are not mature.
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
Zeolite 13X is a mature adsorbent that presents high CO2 adsorption capacity and selectivity, but requires relatively high energy for regeneration and its CO2 adsorption capacity is highly sensitive to moisture  which represents an important drawback for postcombustion applications. The heat of adsorption of CO2 over an activated carbon is ca. 20 kJ/mol  which is almost half of zeolite 13X  and nearly a quarter of Mg-MOF-74 . Activated carbons present a series of advantages that makes them appealing adsorbents for postcombustion applications: low cost, stability under moisture conditions, and ease of regeneration [12,16,27–29]. The production of low-cost activated carbon from biomass residues either by physical or chemical activation is a well-established technology [30–32]. Physical activation is commonly carried out in a two-step process: ﬁrst a carbonaceous precursor is carbonised in inert atmosphere and subsequently the resulting char is partially gasiﬁed with carbon dioxide, steam or air. Usually carbonisation temperature ranges between 673 and 1123 K, and activation temperature between 873 and 1173 K. Chemical activation makes use of dehydrating agents or oxidants (the most common being KOH, NaOH, K2CO3, H3PO4, and ZnCl2), and can be carried out in a single step process at lower temperatures than physical activation. However, the use of chemical products is less desirable in an environmentally friendly scenario. The consumption of easy-to-use single-cup serving coffee capsules has become very popular in the last few years, driving an increasing public concern about the disposal of the used capsules. Nestlé has addressed the subject by providing dedicated capsule collecting points (over 7000 in 15 countries by the end of 2010) with the ﬁnal aim of recycling the aluminium . Waste coffee is separated from the aluminium container and used together with other organic residues to form compost. Although the recovery of the aluminium used to produce the capsules is the most crucial part of this recycling process, the spent coffee grounds might have applications with greater added value than compost production. Of course, spent capsules are not the solely source of coffee grounds. Approximately 20% of the global production of green coffee beans (6.6 million tons in 2001/2002) are used for instant coffee production . For each kg of soluble coffee produced, near 0.91 kg of coffee grounds are obtained . Coffee grounds can be considered pollutant due to its high carbon content, which will consume a high amount of oxygen to degrade. Even more, by simply pilling them up, they can ferment and/or combust spontaneously, so they cannot be disposed without being previously treated . Coffee grounds are usually used as fuel in the boilers of the soluble coffee industry, as they present a heat value similar to that of coal [35,36]. However, it would be highly desirable to ﬁnd alternative sustainable uses of this abundant residue from the food industry. Apart from burning and compost production, coffee grounds can be used for soil remediation, activated carbon production [37–41] or biodiesel production . In the case of the exploitation of coffee grounds for biodiesel production, the resulting solid waste could still be used for the production of activated carbon . Microwave heat treatment in air has been proposed as an energy-saving method for producing low surface area carbonaceous materials that might be useful for basic dye removal . The production of activated carbon from coffee waste by chemical activation with carbonates for later use in industries of environmental engineering or foodstuff is patented . Activated carbons from coffee grounds have also been obtained by chemical activation with phosphoric acid , mixtures of phosphoric acid and zinc chloride , and potassium hydroxide . In the present work two different methods are studied for the production of low-cost carbon adsorbents from spent coffee grounds: chemical activation with KOH and physical activation with CO2. The properties of the ﬁnal carbons depend on the preparation conditions: activating agent, temperature, and length
of the treatment. Focus was made in developing the narrow microporosity as this has proven to be the key factor in maximising CO2 adsorption capacity in postcombustion conditions . The texture of the carbons was characterised by physical adsorption, and their CO2 adsorption capacity in pure CO2 ﬂow was evaluated between 298 and 373 K by means of a thermogravimetric analyser. Moreover, adsorption/desorption cycles in pure CO2 and N2, and also in diluted CO2/N2 and CO2/He streams were carried out to prove the high selectivity, stability and ease of regeneration of these materials. 2. Materials and methods Spent NespressoÒ coffee grounds (from now on referred to as N) were used as the starting material for the development of activated carbons through two different methods: physical activation with CO2 and chemical activation with KOH. Prior to any treatment, the spent coffee grounds were disposed in large trays and dried in a forced-air convection oven at 373 K for 4 h. The proximate and ultimate analyses are shown in Table 1. Table 2 summarises the experimental conditions of the activation processes carried out. To compare the different activation methods, the carbon yield was calculated and referred to the mass of dry coffee grounds (Table 3). 2.1. Activation with KOH Prior to carry out the activation with KOH, a batch of 20 g of spent coffee grounds were carbonised in a ceramic reactor (i.d. 27 mm) inside a horizontal tube furnace (Carbolite) at 673 K under nitrogen ﬂow (50 cm3 min 1) to reduce the volatile matter content of the starting material. To carry out the activation, 1 g of this lowtemperature char (NCL) was placed forming a ﬁne ﬁlm over a ceramic tray, and covered with a layer of solid KOH. The mixture was then heated at 5 K min 1 up to 673 K under 300 cm3 min 1 of nitrogen ﬂow in a GSM type furnace from Carbolite. This temperature was held for 1 h to allow KOH to melt, dehydrate and mix intimately with the coffee char . Activation was completed by heating the mixture up to 873 K under 300 cm3 min 1 of nitrogen ﬂow, and holding this temperature for 1 h. After cooling down in nitrogen ﬂow, the samples were thoroughly washed with distilled water until neutral pH was attained, and dried at 383 K for 24 h in a forced-air convection oven. Several weight ratios KOH/char were used: 1, 2, 3 and 4. The chemically activated samples were denoted as NCLKy, where y accounts for the KOH/char ratio used. It was also intended to activate the coffee grounds in a single stage, departing directly from the coffee grounds (N) instead of the low-temperature carbonised product (NCL), but the obtained carbon yields were excessively low (results not shown). The effect of activation temperature was also assessed at a ﬁxed KOH/char ratio of 3. Only the results for the sample obtained at 973 K are presented (NCLK3b), due to the low carbon yield obtained at 1073 K. 2.2. Activation with CO2 Prior to carry out the activation with CO2, a batch of 20 g of spent coffee grounds were carbonised in a ceramic reactor (i.d. Table 1 Proximate and ultimate analyses of the NespressoÒ coffee grounds (N) and the carbonised products at 673 and 873 K (NCL and NCH, respectively). Sample
N NCL NCH
Proximate analysis (%, db)
Ultimate analysis (%, daf)
82.9 24.9 4.5
1.3 3.4 14.6
56.4 81.2 86.3
7.0 3.7 2.5
2.6 4.8 4.9
34.0 10.3 6.3
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
Table 2 Description of the activation conditions used to produce activated carbons from spent coffee grounds. Sample
Precursor Temperature (K)
KOH/ Heating char rate 1 (K min ) (weight ratio)
Gas Flow rate (cm3 min 1)
NCLK1 NCLK2 NCLK3 NCLK4 NCLK3b NCHA29 NCHA36 NCHA41
NCL NCL NCL NCL NCL NCH NCH NCH
5 5 5 5 5 25 (N2) 25 (N2) 25 (N2)
N2 N2 N2 N2 N2 CO2 CO2 CO2
873 873 873 873 973 973 973 973
1 2 3 4 3 – – –
300 300 300 300 300 10 10 10
Table 3 Carbon yield, point of zero charge and helium density of the samples. Sample
Yield (g/ 100 g N)
Helium density (g cm 3)
N NCL NCH NCLK1 NCLK2 NCLK3 NCLK4 NCLK3b NCHA29 NCHA36 NCHA41
100 29 23 7 12 13 15 9 16 15 14
1.37 1.31 1.44 1.76 1.57 1.55 1.79 2.10 1.89 1.72 1.83
5.2 8.6 9.6 7.6 7.4 7.9 7.9 8.4 9.9 10.1 10.0
27 mm) inside a horizontal tube furnace at 873 K under nitrogen ﬂow (50 cm3 min 1). This temperature is sufﬁcient to produce a high quality charcoal with reduced volatile matter content (see Fig. 1 and Table 1). The resulting char (NCH) was then activated at 973 K using a carbon dioxide ﬂow of 10 cm3 min 1 in batches of around 3 g in a double jacket quartz reactor (i.d. 20 mm) inside a vertical tube furnace up to three different burn-off degrees (deﬁned as the g lost during activation per 100 g of initial char): 29%, 36% and 41%. The samples will be referred to as: NCHA29,
Fig. 1. Pyrolysis of NespressoÒ coffee grounds in 50 cm3 min heating rate of 15 K min 1.
of nitrogen ﬂow at a
NCHA36 and NCHA41, respectively. The activation conditions were selected according to the results of a non-isothermal reactivity test carried out in a thermogravimetric analyser under CO2 ﬂow, and the research group experience [47–49]. Higher burn-off degrees were avoided to prevent the widening of the micropores. These activation conditions (low CO2 ﬂowrate and moderate temperature and burn-off) promote homogeneous gasiﬁcation throughout the whole porous structure and the desired texture development in the micropore domain. 2.3. Characterisation The density of the samples was measured through helium picnometry at 308 K in an Accupyc 1330 from Micromeritics. The acid/basic character of the obtained carbons was assessed by measuring the pH of carbon suspensions in equilibrium with distilled water under inert atmosphere: the average pH for the suspensions with 10–18 wt.% solid is taken as the pHPZC . The morphology of the samples was studied by Scanning Electron Microscopy (SEM) using a FEI Quanta™ 650 FEG. The scarce inorganic matter found in the backscattered electron images was analysed by Energy Dispersive X-ray microanalysis (EDX). The porous texture of the samples was characterised by physical adsorption of N2 and CO2 at 77 and 273 K, respectively, in a TriStar 3000 apparatus from Micromeritics. Prior to adsorption measurements, the samples were evacuated overnight at 373 K. CO2 adsorption at 273 K allows the assessment of narrow microporosity (below 1 nm) whereas N2 adsorption at 77 K covers wider porosity. The micropore volume was determined making use of the Dubinin–Radushkevich (DR) equation assuming an afﬁnity coefﬁcient of 0.34 for N2 and 0.36 for CO2 . The average micropore width (L) was calculated through the Stoeckli–Ballerini equation . The total pore volume (Vp) was calculated from the amount of N2 adsorbed at a relative pressure of 0.99, and the BET surface area from the Brunauer–Emmett–Teller equation . 2.4. CO2 adsorption measurements The CO2 adsorption capacity of the materials at 298 K and atmospheric pressure was assessed by means of a thermobalance TGA92, from Setaram, in pure CO2 ﬂow . Prior to the adsorption measurements the samples were dried in 50 cm3 min 1 of Ar ﬂow at 373 K for 1 h, and then allowed to cool down to 298 K. The CO2 adsorption capacity is assessed from the mass gain experienced by the sample when the gas is switched from Ar to CO2, and is expressed in terms of mmol of CO2 adsorbed per g of dry carbon. To assess the effect of temperature upon the CO2 capture performance, the furnace temperature was raised at 0.5 K min 1 up to 373 K under CO2 ﬂow once the adsorption equilibrium was attained at 298 K. The cyclic behaviour of selected adsorbents was evaluated in a thermogravimetric analyser TGA/DSC1 STARe System from Mettler Toledo. After an initial conditioning step carried out in 100 cm3 min 1 of helium at 373 K for 1 h, the samples were subjected to adsorption and desorption cycles at a constant temperature of 323 K and at atmospheric pressure. Adsorption/desorption cycles were carried out by switching automatically the feed gas between helium and the desired adsorbate each 30 min. Four different feed compositions were studied: 100% CO2, 100% N2, 10% CO2 in He and 10% CO2 in N2. Due to the use of mixtures (multicomponent adsorption) the mass uptake is expressed as percentage. For each cycle, the initial mass (by the end of the previous desorption step in helium) was taken as reference; thus the value presented here refers to the working capacity of the adsorbent in the evaluated conditions.
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
3. Results and discussion Fig. 1 represents the pyrolysis of the starting coffee grounds under N2 ﬂow at a heating rate of 15 K min 1. Adsorbed water is released at near 400 K. The greater mass loss takes place between 500 and 800 K, corresponding to the decomposition of volatiles present in the biomass. In this temperature range two maxima can be differentiated: the ﬁrst at near 600 K, due to the decomposition of hemicellulose, with an elbow ca. 630 K attributed to cellulose, and the second at near 680 K due to the decomposition of lignin, which will be the main contributor to the ﬁnal mass of the char . The small and progressive mass loss above 800 K is due to the char consolidation. Oxygen rich feedstocks, with high hemicellulose and cellulose contents, such as the present case, are expected to lead to carbons with a predominantly microporous structure [56,57], which is highly desirable for the adsorption of carbon dioxide. The starting NespressoÒ coffee grounds present very low ash content (see Table 1), thus showing an adequate precursor for developing activated carbons. The volatile matter content is above 80 wt.%, which is typical for lignocellulosic materials commonly used in the preparation of activated carbons [32,47,48]. The spent coffee grounds present a mild acidic surface, related with its elevated oxygen content. The elemental analysis is in good agreement with published values for coffee grounds from different origins [35,39]. The EDX microanalysis of the ash showed variable amounts of Ca, Al, K, Si, and P and lesser amounts of Mg, Fe and Na. Carbonisation increases the carbon content of the samples, due to the decomposition of hemicellulose, cellulose and lignin, rich in oxygen and hydrogen. Increasing carbonisation temperature from 673 to 873 K decreases the carbon yield from 29% to 23%, due to further primary decomposition of the biomass volatiles (mainly lignin in this temperature range) and through the secondary decomposition and stabilisation of the char . The carbonised coffee grounds present a basic surface with a nitrogen content of near 5 wt.%, which are a priori suitable properties for the adsorption of CO2 [47,48,58–60]. The SEM images of the samples are shown in Fig. 2. The release of volatiles leads to a progressively less dense morphology, accompanied by a reduction in particle size. In the images it can be appreciated that physical activation preserves the morphology of the starting char whereas chemical activation causes substantial particle shrinkage. This effect has also been observed in the SEM images from other KOH biomass-based activated carbons . Backscattered electron images showed scarce mineral matter in all the studied samples, and the EDX analysis showed no higher potassium concentration for sample NCLK3. The carbon yield, helium density and pHPZC of the materials are summarised in Table 3. The carbon yield of the chemically activated samples increased with the ratio KOH/char used at 873 K, but decreased by increasing the temperature for a ratio KOH/char of 3. The carbon yield of physical activation decreases with the burn off attained; that is, with the length of the treatment. For the burn off degrees considered, up to 41%, the yield of physical activation is similar or slightly above that of the chemical activation. Activation increases the density of the carbons due to the preferential elimination of the disorganised carbon that blocks the entrance of the internal porosity of the chars, and also to the break of bonds and the removal of cross-links and carbon atoms which facilitate the atomic rearrangement and thus the densiﬁcation of the material. Densiﬁcation is favoured with increasing temperature, as can be seen from comparison between samples NCLK3 and NCLK3b. For a given temperature, 973 K, chemical activation leads to denser carbons (NCLK3b) than physical activation (NCHA series). This could be a consequence of the greater particle
shrinkage produced by chemical activation. From Table 3 it can also be seen that activation with CO2 increases slightly the basicity of the carbon surface, leading to basic carbons, whereas samples treated with KOH are only slightly basic, with near neutral pHPZC. The increase in pH observed for sample NCHA29 compared to that of char NCH can be attributed to the fact that the activation temperature is 100 K above that of carbonisation. The pH increase with burn off is probably due to formation of basic oxygen surface complexes during the activation process . The lower pH observed for NCLK series compared to NCH and NCL might be attributed to the formation of acidic oxygen groups (R–COOH and R–OH) during KOH activation . Figs. 3 and 4 show the adsorption isotherms of N2 and CO2 at 77 and 273 K, respectively. The shape of the N2 adsorption isotherms and the nearly absence of hysteresis loops point out that all the carbons are essentially microporous. This is highly desirable, as the micropore volume is intrinsically related to the CO2 adsorption capacity at atmospheric pressure . NCL char presents almost negligible N2 adsorption due to diffusion limitations at this temperature; however its incipient microporosity results accessible to CO2 at 273 K. Char NCH, obtained at higher temperature, presents already accessible porosity to the N2 molecule at 77 K. The samples activated with CO2 (NCHA series) present an intermediate texture development between the NCH char and the samples activated with KOH (NCLK series), as can be seen from the amount adsorbed of N2 and CO2. CO2 gasiﬁes the carbon, removing ﬁrst the most reactive carbon deposits formed during carbonisation and then developing the microporosity of the initial char, NCH. The porosity formed upon KOH activation is believed to be due to the intercalation of potassium compounds in the carbon matrix that causes the separation and deformation of the lamellae . These compounds are removed during the washing step leading to permanent porosity. Carbon can also be consumed in this process by potassium reduction and through gasiﬁcation with evolved gases . Table 4 summarises the textural parameters obtained from the analysis of the previously presented adsorption isotherms. It can be observed that the micropore volume (VDR) is in general very close to the total pore volume (Vp); moreover, most of the developed porosity falls in the narrow microporosity domain (with the exception of sample NCLK3b). The average micropore widths calculated from the N2 adsorption isotherm (LDR) are close to 1 nm (with the exception of samples NCH and NCLK3b). As expected, the pore size widens with the burn off degree for physical activation (NCHA series). No signiﬁcant differences were observed in the pore volume or pore size by changing the KOH/Char ratio at 873 K. However, an increase in temperature during KOH activation from 873 to 973 K leads to higher BET surface area and total pore volume, formed by wider porosity (see the broader knee of the N2 adsorption isotherm of sample NCLK3b in Fig. 3 and the linear shape of its CO2 adsorption isotherm in Fig. 4). This effect has been previously described . Although higher BET surface areas have been reported for activated carbons obtained from coffee grounds activated with KOH at 1073 K , this work focuses on the development of the narrow microporosity to maximise CO2 adsorption. The BET surface areas of the chemically activated samples presented in this work (831–1082 m2 g 1) can be favourably compared to activated carbons produced from coffee grounds by chemical activation with H3PO4  and mixtures of ZnCl2 and H3PO4 . The narrow micropore volume (W0), and narrow micropore width (L0) assessed from the CO2 adsorption isotherms at 273 K by the DR method are also presented in Table 4. Both values are higher for the chemically activated samples, with the exception of NCLK3b, which presents a lower volume of narrow micropores, probably due to the collapse of pore walls at the higher temperature that leads to wider pores.
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
Fig. 2. SEM images of: (a) dried spent coffee grounds (N), (b) char carbonised at 673 K (NCL), (c) char carbonised at 873 K (NCH), (d) carbon activated with KOH (NCLK3), and (e) carbon activated with CO2 (NCHA29).
Fig. 3. Adsorption isotherms of N2 at 77 K for the studied samples. Fig. 4. Adsorption isotherms of CO2 at 273 K for the studied samples.
Table 5 summarises the CO2 adsorption capacity of the samples at 273 and 298 K in pure CO2 at atmospheric pressure. A commercial peat-based steam-activated carbon used for CO2 adsorption, R2030CO2 from Norit, has also been included for reference purposes. The carbons obtained from NespressoÒ coffee grounds present CO2 adsorption capacities up to 4.8 mmol g 1 at 273 K, and 3.0 mmol g 1 at 298 K, which are above that of the reference carbon. Samples activated with KOH present the largest CO2 adsorption capacities, followed by the samples activated with CO2 that are in the order of the reference carbon (slightly higher at 298 K). The chars present lower adsorption capacities due to their poor textural development. Note that although NCLK3b is the sample with the greatest adsorption capacity at 273 K, this does not hold at 298 K. As temperature increases (and so the kinetic energy of the gas molecules) only the narrower pores are useful for the adsorption of CO2. Fig. 5 shows the results from the non-isothermal capture tests carried out in the thermogravimetric analyser: when temperature
is raised slowly from 298 to 373 K in CO2 ﬂow, the amount of CO2 that remains adsorbed on the different samples falls from 2 to 3 mmol g 1 to a value close to 0.6 mmol g 1 due to the exothermic nature of the physisorption process. Note that the amount of CO2 adsorbed on series NCHA seems to be less sensitive to the slow heating than that of series NCLK. This implies that the adsorbent–adsorbate interactions are stronger for the samples activated with CO2. This can be attributed to their narrower porosity and their greater surface basicity. Sample NCLK3 was subjected to cyclic adsorption/desorption experiments at 323 K and atmospheric pressure. These conditions can be considered representative of a postcombustion capture process. The corresponding results are summarised in Fig. 6: note that the ﬁrst adsorption step (cycle 0) departs from a different initial state (after the conditioning step at 373 K) and so differs from the following cycles. A cyclic steady state is progressively reached,
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
Table 4 Textural parameters of the samples obtained from the N2 and CO2 adsorption isotherms. Sample
N2 adsorption at 77 K SBET (m2 g
NCL NCH NCLK1 NCLK2 NCLK3 NCLK4 NCLK3b NCHA29 NCHA36 NCHA41
– 84 831 876 840 925 1082 593 568 590
VDR (cm3 g
– 0.03 0.34 0.36 0.34 0.38 0.44 0.24 0.24 0.24
CO2 adsorption at 273 K LDR (nm)
– 2.1 1.1 1.0 1.0 1.1 3.0 0.8 1.0 1.3
0.01 0.04 0.41 0.40 0.37 0.42 0.51 0.24 0.24 0.28
W0 (cm3 g
0.09 0.14 0.41 0.36 0.36 0.33 0.22 0.25 0.25 0.27
L0 (nm) 0.6 0.5 0.6 0.6 0.6 0.6 0.6 0.5 0.5 0.6
SBET: surface area calculated by the BET equation; VDR: micropore volume determined by the DR equation from the N2 adsorption isotherm at 77 K; LDR: average micropore width calculated through the Stoeckli–Ballerini equation; Vp: total pore volume calculated from the amount of N2 adsorbed at 77 K at a relative pressure of 0.99; W0: narrow micropore volume determined by the DR equation applied to the CO2 adsorption isotherm at 273 K; L0: width of narrow micropores calculated through the Stoeckli–Ballerini equation.
Table 5 CO2 adsorption capacity of the samples at 298 K and 101 kPa. Sample
NCL NCH NCLK1 NCLK2 NCLK3 NCLK4 NCLK3b NCHA29 NCHA36 NCHA41 R2030CO2
CO2 adsorption capacity (mmol g 273 K
1.2 2.0 4.9 4.4 4.7 4.5 3.2 3.5 3.4 3.6 3.7
0.8 1.4 2.8 3.0 3.0 2.9 2.7 2.2 2.3 2.4 2.1
Fig. 5. Amount of CO2 that remains adsorbed over the studied samples in pure CO2 ﬂow under a heating rate of 0.5 K min 1.
in which the mass uptake during the adsorption step equals that released during the desorption step. As expected, the mass uptake is maximum when the sample is exposed to pure CO2 ﬂow, reaching a steady value of 7.3 wt.% (equivalent to 1.66 mmol CO2 g 1)
Fig. 6. Adsorption/desorption cycles carried out at 323 K on NCLK3, using helium as purge gas during conditioning and desorption steps, and 100% CO2 (red thick line), 100% N2 (blue ﬁne line), 10% CO2 diluted in N2 (green dots) or 10% CO2 diluted in He (violet dashed line) as the feed gas during the adsorption step. (For interpretation of the references to colours in this ﬁgure legend, the reader is referred to the web version of this article.)
from cycle 3 onwards. The mass uptake when the sample is exposed to pure N2 ﬂow is substantially smaller: 0.9 wt.% (or 0.3 mmol N2 g 1). The ratio of the adsorption capacities of the pure components at atmospheric pressure is usually taken as a rough estimation of selectivity. The resulting CO2/N2 value for NCLK3 is 5 (molar basis). However, in the ﬂue gas the CO2 represents ordinarily between 3% and 15% by volume, being the main diluent N2. Therefore, to assess the adsorption behaviour in a ﬂow with reduced partial pressure of CO2, more representative of the postcombustion conditions, two different cyclic experiments were carried out: the ﬁrst with a feed gas consisting in 10% CO2 in helium, and the second with 10% CO2 in nitrogen. Obviously, in both cases the mass uptake experienced by the sample is well below that undergone in pure CO2 ﬂow due to the reduction in the partial pressure. When the diluting gas is helium (considered inert) the mass uptake (1.9 wt.%) is slightly below that experienced under nitrogen dilution (2.4 wt.%). This indicates that N2 is coadsorbed with CO2. Assuming that the amount of CO2 adsorbed is independent of the nature of the diluting gas (only function of the partial pressure of CO2), the amount of N2 coadsorbed can be estimated by difference. A more adequate estimation of selectivity is that given by the separation factor, deﬁned as the ratio of the molar fractions in the adsorbed phase to that of the gas phase [27,66]. The resulting CO2/N2 selectivity for sample NCLK3 is 13 at cyclic steady state (cycles 3–5). The same protocol was followed for sample NCHA29 (see Fig. 7). Note that although the working capacity in pure CO2 is smaller compared to that of NCLK3 (6.6 vs. 7.3 wt.%), the difference seems to diminish at lower partial pressure of CO2 (1.8 vs. 1.9 wt.% for CO2 diluted in helium and 2.2 vs. 2.4 wt.% when the diluting agent used is nitrogen). The calculated CO2/N2 selectivity of NCHA29 is higher than that of NCLK3: 6 vs. 5 if the data from pure component adsorption are used directly, and 18 vs. 13 using the proper deﬁnition of the separation factor and the data from the experiments with 10% CO2. The higher CO2/N2 selectivity of NCHA29 compared to that of NCLK3 can be attributed to the narrower microporosity and/or the more basic character of the physically activated samples. These results, together with the environmental constraints associated to chemical activation, and the higher carbon yield of physical activation for low burn off degrees, encourages the use of physical activation for the production of CO2 adsorbents from coffee wastes. Future work will involve testing the materials in a ﬁxed-bed adsorption unit to further study the multicomponent adsorption
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
Fig. 7. Adsorption/desorption cycles at 323 K on CNHA29, using helium as purge gas during conditioning and desorption steps, and 100% CO2 (red thick line), 100% N2 (blue ﬁne line), 10% CO2 diluted in N2 (green dots) or 10% CO2 diluted in He (violet dashed line) as the feed gas during the adsorption step. (For interpretation of the references to colours in this ﬁgure legend, the reader is referred to the web version of this article.)
equilibrium and kinetics. Cyclic performance under different regeneration conditions: vacuum swing adsorption and/or temperature swing adsorption will also be evaluated . 4. Conclusions In this work low-cost microporous carbons were produced departing from spent NespressoÒ coffee grounds through physical and chemical activation. The obtained carbons presented CO2 adsorption capacities up to 4.8 mmol g 1 at 273 K, and 3.0 mmol g 1 at 298 K, which are above that of a commercial activated carbon taken as reference. Samples activated with KOH showed superior textural development than samples activated with CO2. For KOH activation it was found that an increase in the activation temperature increased the wide micro- and mesopore volume of the sample at the expense of the ultramicroporosity. Adsorption experiments carried out with pure CO2 at atmospheric pressure showed that activation with KOH leads to higher CO2 adsorption capacities than activation with CO2 due to the superior texture development of the chemically activated samples. However, multicomponent adsorption/desorption cyclic tests carried out at 323 K pointed out that the physically activated samples might be more selective towards CO2 in postcombustion conditions. Moreover, physical activation presents higher carbon yield than chemical activation for low burn off degrees, and also a lower environmental impact (part of the separated CO2 could even be used for activated carbon production). Acknowledgements Work carried out with ﬁnancial support from the Spanish MICINN (Project ENE2008-05087). A.S.G. acknowledges a contract from the MICINN (FPI program), co-ﬁnanced by the European Social Fund. References  Olivier JGJ, Janssens-Maenhout G, Peters JAHW, Wilson J. Long-term trend in global CO2 emissions – 2011 report. The Hague: PBL Netherlands Environmental Assessment Agency, European Union; 2011.  IEA. Carbon capture and storage.
[14.11.11].  Li S, Zhang X, Gao L, Jin H. Learning rates and future cost curves for fossil fuel energy systems with CO2 capture: Methodology and case studies. Appl Energy 2012;93:348–56.
 Hoffmann BS, Szklo A. Integrated gasiﬁcation combined cycle and carbon capture: a risky option to mitigate CO2 emissions of coal-ﬁred power plants. Appl Energy 2011;88:3917–29.  IPCC. IPCC special report on carbon dioxide capture and storage. Cambridge, United Kingdom and New York, NY, USA: IPCC; 2005. p. 442.  IEA, UNIDO. Technology roadmap – carbon capture and storage in industrial applications. International Energy Agency, United Nations Industrial Development Organizations; 2011.  Finkenrath M. Cost of postcombustion carbon dioxide capture from power generation. In: I.E.A. IEA, editor. Paris Cedex: IEA, International Energy Agency; 2011.  Figueroa JD, Fout T, Plasynski S, McIlvried H, Srivastava RD. Advances in CO2 capture technology – the U.S. Department of Energy’s Carbon sequestration program. Int J Greenh Gas Control 2008;2:9–20.  Olajire AA. CO2 capture and separation technologies for end-of-pipe applications – a review. Energy 2010;35:2610–28.  Huang B, Xu S, Gao S, Liu L, Tao J, Niu H, et al. Industrial test and technoeconomic analysis of CO2 capture in Huaneng Beijing coal-ﬁred power station. Appl Energy 2010;87:3347–54.  Malek A, Farooq S. Hydrogen puriﬁcation from reﬁnery fuel gas by pressure swing adsorption. AIChE J 1998;44:1985–92.  Sircar S, Golden TC, Rao MB. Activated carbon for gas separation and storage. Carbon 1996;34:1–12.  Davidson RM. Post-combustion carbon-capture solid sorbents and membranes. In: I.C.C. Centre, editor. International Energy Agency (IEA); 2009.  Sjostrom S, Krutka H. Evaluation of solid sorbents as a retroﬁt technology for CO2 capture. Fuel 2010;89:1298–306.  Ho MT, Allinson GW, Wiley DE. Reducing the cost of CO2 capture from ﬂue gases using pressure swing adsorption. Ind Eng Chem Res 2008;47:4883–90.  Radosz M, Hu X, Krutkramelis K, Shen Y. Flue-gas carbon capture on carbonaceous sorbents: toward a low-cost multifunctional carbon ﬁlter for ‘‘green’’ energy producers. Ind Eng Chem Res 2008;47:3783–94.  Zou Y, Rodrigues AE. Adsorbent materials for carbon dioxide. Adsorpt Sci Technol 2001;1(9):255.  Chaffee AL, Knowles GP, Liang Z, Zhang J, Xiao P, Webley PA. CO2 capture by adsorption: materials and process development. Int J Greenh Gas Control 2007;1:11–8.  Yazaydın AOzr, Snurr RQ, Park T-H, Koh K, Liu J, LeVan MD, et al. Screening of metal–organic frameworks for carbon dioxide capture from ﬂue gas using a combined experimental and modeling approach. J Am Chem Soc 2009;131:18198–9.  Choi S, Drese JH, Jones CW. Adsorbent materials for carbon dioxide capture from large anthropogenic point sources. ChemSusChem 2009;2:796–854.  Hedin N, Chen L, Laaksonen A. Sorbents for CO2 capture from ﬂue gas-aspects from materials and theoretical chemistry. Nanoscale 2010.  Samanta A, Zhao A, Shimizu GKH, Sarkar P, Gupta R. Post-combustion CO2 Capture Using Solid Sorbents – A Review. Ind Eng Chem Res 2012;51:1438–63.  F. Akhtar, L. Andersson, N. Keshavarzi, L. Bergström, Colloidal processing and CO2 capture performance of sacriﬁcially templated zeolite monoliths. Appl Energy, in press.  Himeno S, Komatsu T, Fujita S. High-pressure adsorption equilibria of methane and carbon dioxide on several activated carbons. J Chem Eng Data 2005;50:369–76.  Cavenati S, Grande CA, Rodrigues AE. Adsorption equilibrium of methane, carbon dioxide, and nitrogen on zeolite 13X at high pressures. J Chem Eng Data 2004;49:1095–101.  Bao Z, Yu L, Ren Q, Lu X, Deng S. Adsorption of CO2 and CH4 on a magnesiumbased metal organic framework. J Colloid Interface Sci 2011;353:549–56.  Yang RT. Gas separation by adsorption processes. London: Imperial College Press; 1997.  Siriwardane RV, Shen M-S, Fisher EP, Poston JA. Adsorption of CO2 on molecular sieves and activated carbon. Energy Fuels 2001;15:279–84.  Plaza MG, Pevida C, Arias B, Casal MD, Martín CF, Fermoso J, et al. Different approaches for the development of low-cost CO2 adsorbents. J Environ Eng 2009;135:426–32.  Rodríguez-Reinoso F, Molina-Sabio M. Activated carbons from lignocellulosic materials by chemical and/or physical activation: an overview. Carbon 1992;30:1111–8.  Bansal RC, Goyal M. Activated carbon adsorption. Boca Raton, FL: CRC Press; 2005.  Ioannidou O, Zabaniotou A. Agricultural residues as precursors for activated carbon production – a review. Renew Sustain Energy Rev 2007;11:1966–2005.  Nestlé. Perfecting our packaging solution. [cited 11.11.11].  Niro. Coffee. [cited 11.11.11].  Silva MA, Nebra SA, Machado Silva MJ, Sanchez CG. The use of biomass residues in the Brazilian soluble coffee industry. Biomass Bioenergy 1998;14:457–67.  Sprules RK. Coffee-based solid fuel composition. United States Patent US 5910454; 1999.  Reffas A, Bernardet V, David B, Reinert L, Lehocine MB, Dubois M, et al. Carbons prepared from coffee grounds by H3PO4 activation: Characterization and
M.G. Plaza et al. / Applied Energy 99 (2012) 272–279
  
adsorption of methylene blue and Nylosan Red N-2RBL. J Hazard Mater 2010;175:779–88. Evans MJB, Halliop E, MacDonald JAF. The production of chemically-activated carbon. Carbon 1999;37:269–74. Hirata M, Kawasaki N, Nakamura T, Matsumoto K, Kabayama M, Tamura T, et al. Adsorption of dyes onto carbonaceous materials produced from coffee grounds by microwave treatment. J Colloid Interface Sci 2002;254:17–22. Boonamnuayvitaya V, Sae-ung S, Tanthapanichakoon W. Preparation of activated carbons from coffee residue for the adsorption of formaldehyde. Sep Purif Technol 2005;42:159–68. Namane A, Mekarzia A, Benrachedi K, Belhaneche-Bensemra N, Hellal A. Determination of the adsorption capacity of activated carbon made from coffee grounds by chemical activation with ZnCl2 and H3PO4. J Hazard Mater 2005;119:189–94. Kondamudi N, Mohapatra SK, Misra M. Spent coffee grounds as a versatile source of green energy. J Agric Food Chem 2008;56:11757–60. Franca AS, Nunes AA, Oliveira LS. Activated carbons based on solid residues from coffee biodiesel production. J Biotechnol 2008;136:S654–5. Kuo N-W, Wu P-C. King Car Food Industrial Co., Ltd., Taipei (TW). Method for manufacturing activated carbon from coffee waste. United States Patent US 2003/0196954; 2003. Martín CF, Plaza MG, Pis JJ, Rubiera F, Pevida C, Centeno TA. On the limits of CO2 capture capacity of carbons. Sep Purif Technol 2010;74:225–9. Otowa T, Nojima Y, Miyazaki T. Development of KOH activated high surface area carbon and its application to drinking water puriﬁcation. Carbon 1997;35:1315–9. Plaza MG, Pevida C, Martín CF, Fermoso J, Pis JJ, Rubiera F. Developing almond shell-derived activated carbons as CO2 adsorbents. Sep Purif Technol 2010;71:102–6. Plaza MG, Pevida C, Arias B, Fermoso J, Casal MD, Martín CF, et al. Development of low-cost biomass-based adsorbents for postcombustion CO2 capture. Fuel 2009;88:2442–7. Pis JJ, Mahamud M, Pajares JA, Parra JB, Bansal RC. Preparation of active carbons from coal: Part III: activation of char. Fuel Process Technol 1998;57:149–61. Noh JS, Schwarz JA. Estimation of the point of zero charge of simple oxides by mass titration. J Colloid Interface Sci 1989;130:157–64. Dubinin MM. Properties of active carbons. In: Walker J, L P, editors. Chemistry and physics of carbon. New York: Marcel Dekker Inc; 1966. p. 51–120.
 Stoeckli F, Ballerini L. Evolution of microporosity during activation of carbon. Fuel 1991;70:557–9.  Brunauer S, Emmett PH, Teller E. Adsorption of gases in multimolecular layers. J Am Chem Soc 1938;60:309–19.  Plaza MG, Pevida C, Arias B, Fermoso J, Arenillas A, Rubiera F, et al. Application of thermogravimetric analysis to the evaluation of aminated solid sorbents for CO2 capture. J Therm Anal Calorim 2008;92:601–6.  Cagnon B, Py X, Guillot A, Stoeckli F, Chambat G. Contributions of hemicellulose, cellulose and lignin to the mass and the porous properties of chars and steam activated carbons from various lignocellulosic precursors. Bioresour Technol 2009;100:292–8.  Savova D, Apak E, Ekinci E, Yardim F, Petrov N, Budinova T, et al. Biomass conversion to carbon adsorbents and gas. Biomass Bioenergy 2001;21:133–42.  Wigmans T. Industrial aspects of production and use of activated carbons. Carbon 1989;27:13–22.  Plaza MG, Pevida C, Arenillas A, Rubiera F, Pis JJ. CO2 capture by adsorption with nitrogen enriched carbons. Fuel 2007;86:2204–12.  Plaza MG, Rubiera F, Pis JJ, Pevida C. Ammoxidation of carbon materials for CO2 capture. Appl Surf Sci 2010;256:6843–9.  Plaza MG, García S, Rubiera F, Pis JJ, Pevida C. Evaluation of ammonia modiﬁed and conventionally activated biomass based carbons as CO2 adsorbents in postcombustion conditions. Sep Purif Technol 2011;80:96–104.  Tay T, Ucar S, Karagöz S. Preparation and characterization of activated carbon from waste biomass. J Hazard Mater 2009;165:481–5.  Wang Z-M, Kanoh H, Kaneko K, Lu GQ, Do D. Structural and surface property changes of macadamia nut-shell char upon activation and high temperature treatment. Carbon 2002;40:1231–9. ´ az-Terán J, Nevskaia DM, Fierro JLG, López-Peinado AJ, Jerez A. Study of  Dı chemical activation process of a lignocellulosic material with KOH by XPS and XRD. Micropor Mesopor Mater 2003;60:173–81.  Lillo-Ródenas MA, Cazorla-Amorós D, Linares-Solano A. Understanding chemical reactions between carbons and NaOH and KOH: An insight into the chemical activation mechanism. Carbon 2003;41:267–75.  Oh GH, Park CR. Preparation and characteristics of rice-straw-based porous carbons with high adsorption capacity. Fuel 2002;81:327–36.  Ruthven DM, Farooq S, Knaebel KS. Pressure swing adsorption. John Wiley & Sons, Inc.; 1994.  Plaza MG, García S, Rubiera F, Pis JJ, Pevida C. Post-combustion CO2 capture with a commercial activated carbon: comparison of different regeneration strategies. Chem Eng J 2010;163:41–7.